Shock wave studies in solid targets. FAIR Super-FRS production targets Synergy with some targets for other accelerator facilities. Layout of Super-FRS target area. Super-FRS production targets. Slow extraction - ions extracted over few seconds Slowly rotating graphite wheel probably OK
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Shock wave studies in solid targets
FAIR Super-FRS production targets
Synergy with some targets for other accelerator facilities
- ions extracted over few seconds
Fast extraction – the wish list!
→ Instantaneous evaporation of any material
Solid (graphite) target
Liquid Li target
Informal agreement between CCLRC and GSI:
Chris Densham, Mike Fitton, Matt Rooney (CCLRC),
Helmut Weickl, Klaus Sümmerer, Martin Winkler,
Bernhard Franzke (GSI)
R 2 mm
LIFETIME OF THE ROTATING POLYCRYSTALLINE GRAPHITE TARGET CONES
Radiation-induced anisotropic shrinkageof polycrystalline graphite causes deformation of the shape and hence leads to a radial wobble. The radial displacement amplitude R must be 2mm for the operation of the target.
Measured radial displacement rates for the targets made from the graphite grades R6300P and R6400P *)
*) SGL Carbon, D-53170 Bonn, Germany
A new design of graphite wheel. The target cone is subdivided into 12 segments separated by gaps of 1mm at an angle of 45o to the beam direction: This allows unconstrained dimensional changes of the irradiated part of the graphite.
Paul Scherrer Institut • 5232 Villigen PSI ICFA-HB2002 / G. Heidenreich
Expected radiation damage of the target
The approximation formula used by NuMI target group : 0.25dpa/year
MARS simulation : 0.15~0.20 dpa/year
Dimension change …shrinkage by ~5mm in length in 5 years at maximum. ~75mm in radius
Degradation of thermal conductivity …decreased by 97% @ 200 C70~80% @ 400 C
Magnitude of the damage strongly depends on the irradiation temperature.
It is better to keep the temperature of target around400 ~ 800 C
Thermal conductivity (After/Before)
JAERI report (1991)
Toyo-Tanso Co Ltd. IG-11
Long baseline neutrino oscillation experiment
from Tokai toKamioka.
~1GeV nm beam
(100 of K2K)
Super-K: 50 kton
0.75MW 50GeV PS
Distribution of the energy deposit in the target (w/ 1 spill)
Streamlines showing velocity in the helium.
Calc. by John Butterworth
T2K graphite target temperature progression during first 80 seconds
Default acceleration cycle for 50GeV
Total ~3.53s (from TDR)
Idling time is to adjust total power.
If beam loss, power consumption allow,
this can be reduced.
For tantalum c0 = 3414 m/s
Cf: ANSYS implicit wave propagation velocity :
T2K graphite target shock-wave progression over 50 µs after 4.2 µs beam spill, cross-section of long target.
5 μs (end of beam spill)
Max Von Mises Stress:Ansys – 7MPa
LS-Dyna – 8Mpa
Max Longitudinal Stress:Ansys – 8.5MPa
LS-Dyna – 10MPa
Shock wave experiment at RAL
Pulsed ohmic-heating of wires may be able to replicate pulsed proton beam induced shock.
Ta or graphite wire
50kV, ~8kA PSU 50Hz
At ISIS, RAL
Doing the Test
The ISIS Extraction Kicker Pulsed Power Supply
Time, 100 ns intervals
Rise time: ~50 nsVoltage peak: ~40 kVRepetition rate up to 50 Hz.
+ There is a spare power supply available for use.
LS-Dyna calculations for shock-heating of different graphite wire radii using ISIS kicker magnet power supply
Refractive index n
Damage in tantalum wire:
1 hour x 12.5 Hz at 2200K
Repeat with graphite!